epr and dsc study of the decay of allyl macroradicals in ... the decay of allyl macroradicals in...
Post on 24-Jun-2020
Embed Size (px)
EPR and DSC Study of the Decay of Allyl Macroradicals in Chemically Crosslinked Polyethylene
aM. KLÍMOVÁ, bJ. BARTOŠ, and aF. SZÖC3
Polymer Institute, Slovak Academy of Sciences, CS-842 36 Bratislava
bResearch Institute of Rubber and Plastic Technology, CS-764 22 Zlín
Received 6 June 1990
The decay of allyl macroradicals in chemically crosslinked polyethylenes was studied as a function of the chemical crosslinking and temperature by the EPR method. The decay rate constant was found to decrease in the temperature range between 293 and 323 К with the increasing gel fraction until the reaching of stable value at higher crosslinkings. On the other hand, the rate constant for decay increases monotonously with temperature in the region of lower gel fractions but within the region of higher gel contents its increase is stepwise. Dependences of the rate constant on the gel content are closely associated with the struc tural-chemical changes of the amorphous phase caused by the crosslinking of macromolecules. Temperature dependences of the rate constant are influenced by the course of phase change indicated by compensation effect and proved by DSC technique.
The importance of classical polymers which are modified in various physical or, more often, in physicochemical ways is at present increasing . One of the best known polymers is poly ethylene (PE) crosslinkable by radiation or by chemical initiators. It is widely used especially in electrotechnical industry, where not only me chanical and electric properties but also its life time are significant. Generally speaking, the pres ence of radical centres and physicochemical con ditions of the reactions plays a substantial role in chemical ageing of polymers .
The aim of this paper is to investigate in detail the decay of relatively stable allyl macroradicals in crosslinked low-density polyethylene in depen dence on the crosslinking extent and temperature. Some results from this study have been published in a preliminary paper .
Low-density polyethylene PE, Bralen 03-23, p2 0= 0.923 g cm"
3 , /Ww = 1.3 x 10 5, was used.
A series of samples modified by chemical cross- linking w^s prepared from this polymer using dicumyl peroxide (DCP) in amount between 0 and 2.0 mass % in inert N2 atmosphere at 428 К during 5 h. After taking the samples from the annealing bath, they were cooled at laboratory temperature. All samples were evacuated and
gamma-irradiated from Co source at 293 К with a total radiation dose of 20 kGy.
The contents of gel fractions were determined by weighing insoluble portions in nonirradiated and irradiated samples after their extraction in boiling benzene for 20 h.
Thermal characteristics were recorded on a DSC-1B Perkin—Elmer apparatus equipped with an additional cooling circuit. The calibration of the temperature scale of the calorimeter was done by using indium. The measurements were done in an inert atmosphere of gaseous N2 at the heating rate of 16 °C min"1
A Varian E-4 spectrometer was used for ESR measurements. The kinetic measurements of the decay of macroradicals were done using an E-257 temperature equipment. The concentrations of free radicals were obtained by comparing with a Varian Strong Pitch standard and processed on a Varian computer.
Table 1. Gel and Temperature Characteristics for the Series of the Chemically Crosslinked and Gamma-Irradi ated PE
0 0.05 0.2 0.4 0.8 1.5 2.0
0 21.8 57.4 68.9 79.3 84.5 89.4
310 309 307 306 306 305 304
W K 384 383 383 382 381 380 377
20 Chem. Papers 46 (1) 20—23 (1992)
DECAY OF ALLYL MACRORADICALS
RESULTS AND DISCUSSION
Table 1 contains gel and temperature charac teristics of polyethylene as a function of the con tent of crosslinking initiator. Gel fractions of irradi ated samples were taken as a measure of the crosslinking of the amorphous phase of PE matrix.
The EPR spectra of all samples give septet sig nal  belonging to allyl macroradicals of vinylene type . Kinetic measurements of the decay of these free-radical centres were carried out over the temperature range between 293 and 323 K. The time dependences of the total concentrations of free radicals were found to obey the second- order kinetic equation . On this basis we can use a model of the diffusion-controlled reactions in a condensed phase for the interpretation of the decay mechanism
FT+R- ^ (R#R#) К -> P (A)
Here /cm, /c_m, and kr are the rate constants for migration of the reactants into and out of the cage complex and final reaction.
The effective second-order rate constant /ceff is here given by the relation
^eff - km + kr
which, within the limit kx >>/cm, /c_m changes to /ceřf « /cm. In the case of allyl macroradicals, be cause of their thermodynamic stability, km = /cphm, where /cphm is the rate constant for physical mi gration, i.e. for some molecular motion that leads to an approaching of reactants. Table 2 shows the values of the effective rate constants for the decay of allyls and gel fraction at four tempera tures from the mentioned temperature interval. The rate constants for allyl decay decrease at all temperatures with increasing crosslinking and saturate at the highest gel contents for each temperature.
A treatment of temperature variations of the rate constants of the series of polyethylenes studied is based on the application of Arrhenius equa-
Table 2. The Values of the Effective Rate Constants for the Allyl Decay in Chemically Crosslinked PE
• -50.0 -
Fig. 1. Arrhenius plot for allyl decay rate constants in uncrosslinked PE (CJ), and in chemically crosslinked PE with gel content in mass %: • 21.8, О 57.4, © 89.4.
tion (Fig. 1). Table 3 summarizes values of the effective pre-exponential factors /Q,^ and effective activation energies Eeff. Both parameters increase with the increasing gel content. In addition, they are connected in the so-called compensation dependence. Fig. 2 gives the test of the com pensation effect, I.e. linearity between In k0 eff and Eeff. These properties of both parameters may be interpreted in two ways.
Let us assume that the effective values of ki netic parameters characterize the real physico- chemical process of the decay of allyls in a series of samples examined and that they have a physi cal significance. Then it is possible to apply a model of transient state in connection with the concept of the cooperation of elementary reac tions in the condensed phase [5, 6]
*m — . T- n AS
kT s- -fchem+ ПУ
where к is the Boltzmann constant, h the Planck constant, Г the absolute temperature, n the num ber of segments in molecular motion, AS the acti-
Table 3. The Kinetic Parameters of the Allyl Decay and the Estimated Quantities from Lebedev's Model in Chemically Crosslinked PE
0 21.8 57.4 68.9 79.3 84.5 89.4
7= 293 К
7.81 0.49 0.21 0.17 0.13 0.11 0.11
k*C 10"/(д sP'n"1 s"1)
7=303K T=313K T=323K
16.0 31.0 57.9 1.45 2.5 5.1 0.49 1.38 3.1 0.39 1.17 2.65 0.37 0.97 2.4 0.37 0.89 2.4 0.32 0.88 2.3
0 21.8 57.4 68.9 79.3 84.5 89.4
g spin"1 s"1
1.65 x 1 0 й 2
124 x 1 0 й 0
2.00 x 1 0 й 0
5.01 x 10"9
52.3 60.3 71.7 73.5 76.2 792 80.4
kJmor 1 K" 1
0 -0.026 -0.063 -0.069 -0.078 -0.087 -0.091
К g spin-1 s"1
1.65 x 10"12
124x10" 1 3
6.35 x 10"14
5.08 x 10"14
4.17 x 10"14
3.91 x 10"14
Chem. Papers 46 (1) 20—23 (1992) 21
M. KUMOVÄ, J. BARTOŠ, F. SZÖCS
1 60 70
fe f f / (»i and the peak T"m p, respectively. The values of both quantities evidently decrease with the increasing gel content. A comparison of Fig. 3 with Table 1 may lead to the following results. In the case of reference and low-cross- linked sample, the temperature interval of kinetic measurements covers the region of temperatures below and near 7m j. On the other hand, for high- crosslinked samples, as follows from a compari son of the temperature intervals, the acceleration of the decay of allyls correlates with the onset of the melting of the crystalline regions in semicrys- talline matrix. It is thus the transformation of
22 Chem. Papers 46 (1) 20—23 (1992)
the crystalline phase to the amorphous one that speeds up the transport of allyl centres during their decay. This DSC evidence supports conclu sions following from both interpretations of Arrhe- nius parameters. From a microscopic point of view it means that at temperatures 313 К and 323 К the phase transformation, i.e. the decay of crys tallites increases the molecular mobility in the ma trix. Consequently, the rate of migration of allyl macroradicals is in their decay reaction enhanced.
On the basis of the present results from the study of the decay of ally